Crystal plasticity finite element simulations using a plasticity ï¬nite element simulations...
Embed Size (px)
Transcript of Crystal plasticity finite element simulations using a plasticity ï¬nite element simulations...
International Journal of Plasticity 66 (2015) 7184
Contents lists available at ScienceDirect
International Journal of Plasticity
journal homepage: www.elsevier .com/locate / i jp las
Crystal plasticity finite element simulations usinga database of discrete Fourier transforms
http://dx.doi.org/10.1016/j.ijplas.2014.04.0060749-6419/ 2014 Elsevier Ltd. All rights reserved.
Corresponding author. Tel.: +1 2672354208.E-mail address: email@example.com (S.R. Kalidindi).
Hamad F. Alharbi a,b, Surya R. Kalidindi a,a George W. Woodruff School of Mechanical Engineering, Georgia Institute of Technology, Atlanta, GA 30332, USAb Mechanical Engineering Department, King Saud University, PO Box 800, Riyadh 11421, Saudi Arabia
a r t i c l e i n f o
Article history:Received 29 September 2013Received in final revised form 6 March 2014Available online 6 May 2014
Keywords:Crystal plasticityFinite element simulationsDiscrete Fourier transformsMicrostructurePlastic deformation
a b s t r a c t
In recent work, we have demonstrated the viability and computational advantages of usinga compact database of discrete Fourier transforms (DFTs) for facilitating crystal plasticitysolutions in cubic polycrystalline materials subjected to arbitrary deformation paths. Thisnew DFT database approach allows for compact representation and fast retrieval of crystalplasticity solutions, which is found to be able to speed up the calculations by about twoorders of magnitude. In this paper, we present the first successful implementation of thisspectral database approach in a commercial finite element code to permit computationallyefficient simulations of heterogeneous deformations using crystal plasticity theories. Morespecifically, the spectral database approach to crystal plasticity solutions was successfullyintegrated with the commercial finite element package ABAQUS through a user materialsubroutine, UMAT. Details of this new crystal plasticity spectral database-FE approachare demonstrated and validated through a few example case studies for selected deforma-tion processes on face centered and body centered cubic metals. The evolution of theunderlying crystallographic texture and its associated macroscale anisotropic propertiespredicted from this new approach are compared against the corresponding results fromthe conventional crystal plasticity finite element method. It is observed that implementingthe crystal plasticity spectral database in a FE code produced excellent predictions similarto the classical crystal plasticity FE method, but at a significantly faster computationalspeed and much lower computational cost.
2014 Elsevier Ltd. All rights reserved.
Crystallographic texture and its evolution are known to be major sources of anisotropy in polycrystalline metals. Highlysimplified phenomenological models cannot usually provide reliable predictions of the materials anisotropy under complexdeformation paths, and lack the fidelity needed to optimize the microstructure and mechanical properties during the pro-duction process. On the other hand, physics-based models such as crystal plasticity theories have demonstrated remarkablesuccess in predicting the anisotropic mechanical response in polycrystalline metals and the evolution of underlying texturein finite plastic deformation. However, the use of crystal plasticity models is extremely computationally expensive, and hasnot been adopted broadly by the advanced materials development community.
72 H.F. Alharbi, S.R. Kalidindi / International Journal of Plasticity 66 (2015) 7184
Crystal plasticity theories aim to predict the plastic anisotropy of polycrystalline materials by accounting for the funda-mental mechanism of plastic deformation at the scale of the constituent single crystals by taking into account the details ofslip system geometry in each individual crystal. To predict the response of the overall polycrystalline aggregate, one needs touse one of the homogenization models that can be classified based on the assumptions made with regard to the local inter-actions between grains, such as Taylor-type (also known as full constraints) Taylor (1938), relaxed constraints (Kocks andMecking, 2003), LAMEL (Van Houtte et al., 2005), self-consistent (Lebensohn et al., 2004, 2007; Lebensohn and Tom,1993; Molinari et al., 1987), and crystal plasticity finite element (Bachu and Kalidindi, 1998; Kalidindi and Anand, 1994;Kalidindi et al., 1992; Kalidindi and Schoenfeld, 2000; Needleman et al., 1985; Peirce et al., 1982, 1983) models. The simplestand the most widely used approach is the Taylor-type model. In this method, the applied velocity gradient tensor at themicroscale is assumed to be the same as the one applied at the macroscale (on the polycrystal). The macroscopic stressfor the polycrystal is obtained by volume averaging the stresses inside the polycrystal. The Taylor-type model usually pro-vides good predictions of the overall anisotropic stressstrain response and the averaged texture evolution for single-phase,high stacking faulty energy, cubic metals (Bronkhorst et al., 1992b). However, it usually lacks good predictions at the scale ofindividual crystals and it fails to show the development of heterogeneities within the grains (Bhattacharyya et al., 2001;Kalidindi et al., 2004; Van Houtte et al., 2005).
The most sophisticated and successful model that takes into account the local interactions between all grains in the sam-ple is the crystal plasticity finite element method (called CPFEM) (Bachu and Kalidindi, 1998; Kalidindi and Anand, 1994;Kalidindi et al., 1992; Kalidindi and Schoenfeld, 2000; Needleman et al., 1985; Peirce et al., 1982, 1983). This approach usesthe finite element method to find the response of the polycrystal by placing a finite element mesh over the grains such thateach element represents one grain or a part of the grain. The crystal lattice orientations and material state variables areupdated at every integration point in the finite element mesh by solving the crystal plasticity constitutive equations. In thisapproach, the equilibrium and compatibility conditions are satisfied using a weak form of the principle of virtual work. Thismodel not only provides excellent predictions of the texture and anisotropic stressstrain response, but also predicts thelocal lattice rotations and heterogeneity of plastic deformation at the crystal level (Choi et al., 2011; Delaire et al., 2000;Erieau and Rey, 2004; Hripr et al., 2007; Kalidindi et al., 2004; Kanjarla et al., 2010; Musienko et al., 2007; Raabe et al.,2002; Sachtleber et al., 2002; St-Pierre et al., 2008; Zhao et al., 2008). This approach, however, requires very large compu-tational resources because of the high computational time required to solve the highly nonlinear, numerically stiff, crystalplasticity constitutive equations at every integration point. This makes the use of CPFEM impractical when the size of thepolycrystalline aggregate is very large. It should be noted that when using CPFEM for large-scale applications such as metalforming operations, a representative polycrystalline microstructure needs to be assigned to each integration point in the FEmodel. In this case, a suitable homogenization approach needs to be employed to obtain the mechanical behavior of the poly-crystalline aggregate at each material point. The execution of such simulations becomes computationally prohibitive if themodel consists of a large number of elements. Several approaches have been developed to improve the computational effi-ciency of these simulations (see, e.g., (Luo and Rousselier, 2014; Raabe and Roters, 2004; Raabe et al., 2004; Rousselier et al.,2012; Tikhovskiy et al., 2007; Zhao et al., 2008)). The recently developed crystal plasticity fast Fourier transform (CPFFT)method offers a promising alternative approach to CPFEM with periodic boundary conditions (Lebensohn, 2001;Lebensohn et al., 2008; Suquet et al., 2012). This approach has been shown to offer significant computational advantagesthrough the use of an efficient FFT-based algorithm (Liu et al., 2010; Prakash and Lebensohn, 2009).
Several higher-order homogenization models have also been proposed to obtain the response of the polycrystal from theresponses of constituent single crystals. The most widely used approach is the viscoplastic self-consistent model (Lebensohnet al., 2004, 2007; Lebensohn and Tom, 1993; Molinari et al., 1987). The self-consistent approach assumes that each crystalacts as an ellipsoidal inclusion embedded in a homogenous effective medium that has the average behavior of the polycrys-tal. Therefore, the local interaction between each crystal and the neighboring crystals is taken in an average sense over thecomplete polycrystal. On the other hand, the LAMEL model considers the local interactions between immediate neighboringgrains by careful examination of the stress equilibrium at the grain boundaries (Kanjarla et al., 2010; Liu et al., 2002; VanHoutte et al., 2002, 2006, 2005). Numerous studies have been published to compare the predictions from the differenthomogenization methods (see for example (Lebensohn et al., 2003; Van Houtte et al., 2002, 2005)). Van Houtte et al.(2002, 2005) provided quantitative comparisons between different homogenization methods including full-constraints,relaxed constrains, LAMEL, visco-plastic self-consistent, and CPFEM models. The CPFEM is usually used to validate any otherhomogenization model because it accounts for both stress equilibrium and strain compat